A series of new materials of varying chemical and physical properties could be obtained by varying the composition of constituents of binary and ternary semiconductors; in this respect for example newer materials like Pb1-x CdxS, CuInS2, CuInSe2, ZnSSe/ZnSe and ZnCdS can be used for better efficiency1-7. Sulfide and mixed sulfide thin film coating find extensive use in number of electronic devices such as photoconductors, thin film transistors, photo-detectors, electroluminescent cells and photovoltaic devices8-12. Lead sulfide thin films have been deposited by LP-MOCVD and AACVD, using single-source precursors of the type
Study of electrical optical and structural properties
of lead selenide sulphide ternary thin films
S.R. JADHAV¹ and U.P. KHAIRNAR²
¹Department of Physics, Rashtriya College, Chalisgaon, Dist- Jalgaon - 424 101 (India). ²Department of Physics, S.S.V.P.S. ACS College, Shindkheda - 425 406 (India).
(Received: October 04, 2010; Accepted: November 12, 2010)
Polycrystalline Lead Selenide Sulphide thin films have been deposited on glass substrate at 300 K by thermal evaporation technique. The different sets of samples of varying composition ‘x’ from 0.1 to 0.9 were deposited and annealed at reduced pressure of 0.1 micron for duration of 4 hours at temp (373) K. The material parameters determined are bulk resistivity 1.450 (Ohm-cm), mean free path 2820 Å and carrier concentration 5.5 x 1012 per cm3. The estimated activation energy for heating
cycles is larger as compare to cooling cycles. Fermi-energy determine from TEP study are within ranges between band gap energy and activation energy values.
Also the XRD study reveals that all the samples were polycrystalline having cubic FCC, cubic and tetragonal structure. The dependence of absorption coefficient ‘’ on photon energy has been determined. The analysis of result so that for Lead Selenide Sulphide films of different composition, direct transition occurs with band gap energy in the range of 1.0 eV to 1.4 eV. Refractive indices and extinction coefficient have been evaluated and are in the range 1.20 to 4.80 and 0.005 to 0.0245 respectively. The compositions of films were analyzed using Energy Dispersive X-ray Analysis (EDAX). Also the grain size is determined from X-ray diffraction study. Most of the grain sizes are below 300 Å indicates that the film material exhibits nano structure. The SEM analysis indicates that the film is covered with large number of star shaped microgranuals. The size of the microgranuals increases with increasing ‘x’.
Key words: Thermal evaporation, optical constants, XRD, EDAX, SEM.
MATERIAL AND METHODS
For the preparation of ternary compound semiconductors (PbSe)x(PbS)1-x the constituent compounds PbSe and PbS have been taken in molecular stiochiometry proportional weights and crushed and mixed homogeneously. The different sets of samples of varying compositions (x = 0.1 to 0.9) were deposited on to the amor phous precleaned glass substrates at room temperature 308 K. All the samples are deposited under the similar optimized conditions. The thicknesses of films were controlled by using quartz crystal thickness monitor model No. DTM-101 provided by Hind-High Vac. The deposition rate was maintained 10-15 Å/ sec constant throughout sample preparations. These samples were annealed at reduced pressure of 0.1 micron for the duration of 4 hours at the temperature of 373 K and maintained carefully. These samples were then used for different characterizations.
The structural characterization was done by X- ray diffractometer (Rigacu-Miniflex, Japan) with CuK radiation (1.5418Å) and Analytical Scanning Electron Microscope (SEM) JEOL JSM 6360 (LA), with EDAX attachment. The transmittance of the films was determined at normal and near normal incidence of light in the wavelength range 200 to 2600 nm by means of double beam spectrophotometer (Hitachi-330 model).
RESULTS AND DISCUSSION Electrical Properties
Resistivity variation as a function of composition parameter ‘x’ as presented in Fig.1 Seems to be obvious as resistivity of pure material (i.e. x = 0) PbS and PbSe are of value 0.027 -cm and 0.25 -cm respectively. As x increases resistivity should increase and it should be maximum at x = 0.5, theoretically instead of this it is observed that resistivity increases slowly with x up to x = 0.7 and then it rapidly increases up to x = 0.9 For all samples x 0 the resistivity is larger than that of pure material films of same order of thickness around 2000Å13. Similar behavior of resistivity variation for all composition of ‘x’ may be due to similar processes of activation of conductivity of charge carriers may be involved. This behavior in
Table 1: Band gap energies for ternary compound PbSeXPbS1-X Composition Thickness Band gap
‘x’ (d) Å energy Eg (eV)
0.1 1200 1.16
0.2 1450 1.12
0.3 2100 1.04
0.4 1900 1.04
0.5 1850 1.16
0.6 1250 1.43
0.7 1300 1.40
0.8 1450 1.28
0.9 1520 1.16
Table 2: Range of ‘n’ values for the ternary compound PbSex PbS1-x Composition‘x’ Rang of ‘n’ of values
0.1 3.33 – 1.22
0.2 4.56 – 1.22
0.3 4.80 – 1.22
0.4 4.32 – 1.22
0.5 4.44 – 1.22
0.6 3.60 – 1.22
0.7 2.69 – 1.22
0.8 3.89 – 1.22
0.9 3.51 – 1.57
Table 3: Range of ‘k’ values for various compositions of the ternary compound PbSex PbS1-x Composition‘x’ Range of ‘k’ of values
0.1 0.0005 – 0.0245
0.2 0.0014 – 0.0150
0.3 0.0022 – 0.0157
0.4 0.0038 – 0.0164
0.5 0.0036 – 0.0149
0.6 0.0047 - 0.0176
0.7 0.0017 – 0.0169
0.8 0.0010 – 0.0177
the resistivity is supported by different structural phases involved as composition parameter ‘x’ increases. And similar observations have observed by Deshmukh et. al.16 In this study of (CdSe)
x– (PbS)1-x composite thin films.
Mater ial parameters evaluated approximately were bulk resistivity 0 = 1450 × 10-3 -cm, mean free path l0 = 2820Å and carrier concentration n = 5.5x1012/cm3. The carrier concentration evaluated seems to be very low value as compared to the reported value of 1018/ cm3 by Fujita et.al.17 for PbS
0.5 Se0.5 prepared by co-evaporated method on rock salt and PbSx Se1-x single crystal substrates.
For all compositions change in thermoelectric power at low temperature end is appreciably larger and very small changes at high temperature region except the compositions PbSe0.3 S0.7, PbSe0.4 S0.6 and PbSe0.5 S0.5, have appreciable ther moelectric power changes over entire temperature range may be increasing or decreasing. From the Fig. 2–3 fermi energies have been evaluated from the linear variation of thermoelectric power verses reciprocal of temperature. These values are within ranges in between band gap energy values around 1.2 eV and evaluated thermally activation energies (0.24 - 0.44) eV.
The transmittance spectra have
Table 4 EDAX Data for (PbSe)x (PbS)1-x Composite thin films (x = 0.1 to 0.9) (atomic percent)
Composition Atomic Atomic Atomic EDAX Composition
‘x’ Percent Percent Percent Atomic Atomic Atomic
Pb Se S Percent Pb Percent Se Percent S
0.1 50 5 45 - -
-0.2 50 10 40 14.57 3.23 22.71
16.15 8.67 18.64
20.32 3.81 26.44
0.3 50 15 35 46.83 17.36 35.82
46.08 17.94 35.98
48.91 17.99 33.10
0.4 50 20 30 47.21 27.83 24.96
46.42 27.59 25.98
47.05 27.40 25.54
0.5 50 25 25 46.43 21.39 32.18
48.82 21.07 30.11
45.30 33.27 21.42
0.6 50 30 20 38.96 36.59 24.44
38.76 25.88 35.35
39.37 34.21 26.42
0.7 50 35 15 0.00 42.53 57.47
6.51 23.15 70.70
12.02 52.80 35.17
0.8 50 40 10 40.21 44.70 15.09
39.88 44.47 15.65
41.98 44.01 14.01
0.9 50 45 5 38.87 46.27 14.85
38.24 46.79 14.97
Fig. 2: Variation of TEP with reciprocal of temperature for PbSeX PbS1-x thin films (x = 0.1) Fig. 1: Variation of Resistivity as a function of
composition ‘x’ for PbSex PbS1-x (x = 0.1 to 0.9)
Fig. 4: Variation of (hn)2 with photon energy for PbSex PbS1-x thin film (x = 0.8) Fig. 3: Variation of TEP with reciprocal of
temperature for PbSeX PbS1-x thin films (x = 0.9) characteristic feature as a function of wavelength. Few samples are opaque below 750 nm and some of them are opaque below 950 nm. Then the transmittance increases linearly and rapidly with wavelength and attains maximum value. Also in few samples there is a well defined maxima and minima peak from the spectra. The transmittance data have been used to calculate absorption coefficients an attempt is made to plot the curves (hn)2 vs hn and the curve is presented in Fig. 4. All the compositions curves shows linear variations and extended line intersects the hn axis. This intersection gives optical band gap energies. These evaluated values are presented in Table 1. These values are in the range 1.04 – 1.43 eV and varied randomly when composition parameter is less than 0.5 (x 0.6).
Band gap energy ‘Eg’ is maximum for x = 0.6 and it decreases at x > 0.6, for these samples the thickness is also of increasing order and therefore band gap energy is also as expected goes on decreasing order. This fact is also explained for PbSe and PbS films18-21.
Fig. 5: X – Ray Diffractograms of various (PbSe)x (PbS)1-x Structures (x = 0.1 to 0.5) Structural Properties
Table 4 represents the detail EDAX analysis of the composition of starting basic ingredients and film composition comparisons. And
It is seen from this table that the samples of compositions x = 0.3, 0.4 and 0.5 are not much deviated from the expected atomic percentage while the samples with x = 0.6, 0.8 and 0.9 are comparatively more deviated than expected. While the sample of composition x = 0.7 is largely deviated from the expected atomic percentage.
The XRDs of all compositions (0.1 x 0.5) have been presented in Fig. 5. X-ray diffractograms differs for different compositions in relative intensities, angular positions and even relative orientations. The comparison of observed and standard diffraction parameters for three different structures of PbSeS, PbSe and PbS compounds. A detailed comparison indicates that observed and standard ‘d’ values very closely agree with each other for all composition parameters x varying from 0.1 to 0.9. The XRD analysis confirms that film material is polycr ystalline for all compositions.
The relative intensities of prominent reflections of cubic structures of PbSe and F.C.C. structure of PbS (111) (200) and (220). From this table it is observed that, as the compositional parameter x increases, the orientation of crystallites changes from (200) of face centered cubic of PbS to (200) cubic of PbSe.
From the analysis of XRD it is found that the films are of composite structure of PbSe, PbS and PbSeS i.e. cubic face centered, cubic and tetragonal structures. In other words this analysis of different peaks indicating the presence of phases, cubic PbSe, face centered cubic of PbS as well as tetragonal of PbSeS. It is interesting to note that for x = 0.1 – 0.2 face centered cubic face of PbS is prominent than phases of PbSe and PbSeS. For x = 0.4 and 0.5 films are only phase of cubic PbSe and F.C.C. of PbS for x = 0.6 and 0.8 films are constituting all the three phases prominently. For x = 0.9, the films are constitutes tetragonal and cubic phase only, for x = 0.7, the film material is of prominent cubic phase of PbSe only.
In general it may be concluded that film materials of various compositions parameters are of polycrystalline, composite of different phases and having relative crystalline orientation along (200)
of cubic or F.C.C. of PbSe and PbS respectively. L.P.Deshmukh et.al.16, studied composite films of (CdS)x (PbS)1-x grown by chemical bath deposition technique. XRD and microscopic observation show the films were composite and exhibit Phase of cubic and hexagonal (CdS) cubic (CdO) and PbS.
The grain size of crystallites for all the compositions has been evaluated. Most of the values of grain size are below 300 Å which indicates film material exhibit nano-structure.
The film with×4000 magnification for the composition (PbSe)x (PbS)1-x (x = 0.2) at 25 kV accelerating voltage shows the large number of small granules as shown in Fig. 6. But the same film at the low accelerating voltage i.e. 15 kV shows the large number of microgrannuals, but it is interesting to point out that all the granules are star shaped which can be seen from the photographs. This star shape indicates the dendraitic growth of
Fig. 6: Scanning electron micrograph of PbSex PbS1-x thin film (x = 0.2)
the samples. This may be due to the effect of WD changes from 9.3 to 9.6.
is large as compare to x = 0.9 and also their shape is more regular. So for the dendraitic growth of the film is suitable at x = 0.2 (PbSex PbS1-x), but when same film required at sphearolytic shape then x = 0.8 (PbSex PbS1-x) is suitable.
From this we conclude that for x = 0.2 gives the film of dendraitic growth and for x = 0.8 gives the film of sphearolytic shape. Both are in crystalline form and x = 0.2 and x = 0.8 both are having the good quality of the mixed ternary films.
1. Thin films of Polycrystalline Lead Selenide Sulphide were prepared by the thermal evaporation technique.
2. Estimated activation energy for heating cycles is larger as compared to cooling cycles. Also for x < 0.5 the activation energies are of higher magnitudes as compare to x > 0.5.
3. The Estimated values of Fermi-energy determined from thermo electric power study are within ranges between band gap energy and activation energy values.
4. The Band gap energy varies randomly when x < 0.5 and it is systematically decreases when x > 0.6.
5. Detailed X-ray diffraction study reveals that the films are of composite structure i.e. Cubic fcc, Cubic & Tetragonal.
6. Most of the estimated grain sizes are below 300Å. This indicates film material exhibits nano-structure.
7. SEM analysis indicates that the film is covered with large number of star shaped microgrannuals, the size of the microgrannuals increases with increasing ‘x’ when x = 0.8 the microgrannuals are turn on to regular sphearolytic shape and when x = 0.2 film shows dendraitic growth.
The authors are thankful to Prof. Dr. P. H. Pawar, Principal, Z. B. Patil College, Dhule. The authors are also grateful to Prof. Dr. P P. Patil, Director and Head, Depar tment of Physical Sciences, North Maharashtra University, Jalgaon.
1. J.J.Loferski, “Proc. workshop photovoltaic conversion of solar energy for terrestrial application” 1, 27 sponsored by National Science Foundation (USA, 1973).
2. A.K.Sood, K.Wu. and J.N.Zemel, Thin Solid Films, 48: 73 (1978).
3. J.D.Jenes and R.B.Schoolar, Electron. Mater., 7: 237 (1978).
4. A.R.Calwa, J.A.Mroczouski and T.C.Harman, J. Electron Mater., 1: 191 (1972).
5. P. Stitu., Phys. Status Solidi, A15: K19 (1973). 6. Ozden Akinci, H. Hakan Gurel and Hilmi
Unlu, Thin Solid Films, 517: 2431 (2009). 7. Bhaskar Kumar, Parag Vasekar, Shirish A.
Pethe, Neelkanth G. Dhere and Galymzhan T. Koishiyev, Thin Solid Films, 517: 2295 (2009).
8. G. Gordillo, Solar cells, 14: 219 (1985). 9. G.B. Reddy, D.K. Pandya and K.L.Chopra,
Solar Energy Mat., 15: 235 (1987).
10. J.A.Rodriguer and G. Gordillo, Solar energy Mat., 19: 421, (1989).
11. P.K.Nair, M.Ocampo, A. Fernandez and M.T.S.Nair, Solar Energy Mat., 20: 235 (1990).
12. G.C. Morris and R.Vander veen, Solar Energy, Mat. Solar Cells, 26: 217 (1992). 13. T. Trindade and P. O’Brien, Chem. Vap.
Deposition, 3: 75 (1997).
14 N. I. Fainer, M. L. Kosinova, Y. M. Rumyantsev, E. G. Salman and F. A. Kuznetsov, Thin Solid Films, 280: 16 (1996).
15. L.I. Maissel and R. Glang, “Hand Book of Thin Film Technology, Mc Graw – Hill, Book Co. New York, (1970).
16. L.P. Deshmukh, B.M.More, S.G. Ghollkatti and P.P. Hankare, Bull. of Mat. Sci., 17: 455 (1994).
18. T.H. Mayers, S.W. Edwards and J.F. Schetzina, J. Appl. phys., 52: 4231 (1981). 19. N.El. Kadry, M.F. Ahmed and K. Abdel Hady,
Thin Solid Films, 274: 120 (1996).
20. F. Cerdeira, I.T. Torriani, P. Mostisuke, V.
Lemos and F. Decker, Appl. Phys, A 46: 107 (1988).